LMucko/crystallography-open-database huggingface dataset:
Crystal structure of thulium sulfide (5/7), Tm5 S7
Range, K.J.; Rau, F.; Klement, U.; Zeitschrift fuer Kristallographie (149,1979-) 208 (1993) 97–98; doi:

data_8104157
_publ_section_title
;
 Crystal structure of thulium sulfide (5/7), Tm5 S7
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              97
_journal_page_last               98
_journal_volume                  208
_journal_year                    1993
_chemical_formula_sum            'S7 Tm5'
_chemical_name_systematic        'Tm5 S7'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.45
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.455
_cell_length_b                   3.7398
_cell_length_c                   11.268
_cell_volume                     505.888
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Range_ZEKRDZ_1993_1557.cif
_cod_data_source_block           S7Tm5
_cod_database_code               8104157
Crystal structure of deuterides Tb3Ni6Al2Dx (x=0.3,0.5) based on intermetallic Tb3Ni6Al2 with Ca3Ag8 structural type
Yartys', V.A.; Khidirov, I.; Pavlenko, V.V.; Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR)) 18 (1992) 428–435; doi:

data_1536821
_publ_section_title
;
 Crystal structure of deuterides Tb3Ni6Al2Dx (x=0.3,0.5) based on
 intermetallic Tb3Ni6Al2 with Ca3Ag8 structural type
;
_journal_name_full
;
Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR))
;
_journal_page_first              428
_journal_page_last               435
_journal_volume                  18
_journal_year                    1992
_chemical_formula_sum            'Al2 D0.3 Ni6 Tb3'
_chemical_name_systematic        'Tb3 Ni6 Al2 D0.3'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.93
_cell_length_b                   8.93
_cell_length_c                   8.93
_cell_volume                     712.122
_citation_journal_id_ASTM        KOKHDC
_cod_data_source_file            Yartys_KOKHDC_1992_1344.cif
_cod_data_source_block           D0.3Al2Ni6Tb3
_cod_original_formula_sum        'D0.3 Al2 Ni6 Tb3'
_cod_database_code               1536821
Role of bonding, reduced screening, and structure in the hightemperature superconductors
Falter, C.; Klenner, M.; Chen, Q.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 48 (1993) 16690–16706; doi:

data_1536822
_publ_section_title
;
 Role of bonding, reduced screening, and structure in the hightemperature
 superconductors
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              16690
_journal_page_last               16706
_journal_volume                  48
_journal_year                    1993
_chemical_formula_sum            'Cu La2 O4'
_chemical_name_systematic        'La2 (Cu O4)'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-C 2ac 2 (z,x,y)'
_symmetry_space_group_name_H-M   'C m c a (c,a,b)'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.624
_cell_length_b                   5.714
_cell_length_c                   12.198
_cell_volume                     391.989
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Falter_PRBMDO_1993_1893.cif
_cod_data_source_block           Cu1La2O4
_cod_original_cell_volume        391.9893
_cod_original_sg_symbol_H-M      'A b m a'
_cod_original_formula_sum        'Cu1 La2 O4'
_cod_database_code               1536822
Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
Koenigstein, K.; Jansen, M.; Chemische Berichte 127 (1994) 1213–1218; doi:

data_1536823
_publ_section_title
;
 Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
;
_journal_name_full               'Chemische Berichte'
_journal_page_first              1213
_journal_page_last               1218
_journal_volume                  127
_journal_year                    1994
_chemical_formula_sum            'O13 P4 Rb2 Si'
_chemical_name_systematic        'Rb2 Si (P4 O13)'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                83.69
_cell_angle_beta                 83.8
_cell_angle_gamma                81.95
_cell_formula_units_Z            2
_cell_length_a                   4.857
_cell_length_b                   7.717
_cell_length_c                   15.089
_cell_volume                     554.123
_citation_journal_id_ASTM        CHBEAM
_cod_data_source_file            Koenigstein_CHBEAM_1994_1295.cif
_cod_data_source_block           O13P4Rb2Si1
_cod_original_cell_volume        554.1227
_cod_original_formula_sum        'O13 P4 Rb2 Si1'
_cod_database_code               1536823
Crystal structure of ytterbium(III) trisulfide disilicate, Yb4 S3 (Si2 O7)
Range, K.J.; Andratschke, M.; Gietl, A.; Zeitschrift fuer Kristallographie (149,1979-) 211 (1996) 816–816; doi:

data_8104158
_publ_section_title
;
 Crystal structure of ytterbium(III) trisulfide disilicate, Yb4 S3 (Si2
 O7)
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              816
_journal_page_last               816
_journal_volume                  211
_journal_year                    1996
_chemical_formula_sum            'O7 S3 Si2 Yb4'
_chemical_name_systematic        'Yb4 S3 (Si2 O7)'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.543
_cell_length_b                   11.543
_cell_length_c                   13.322
_cell_volume                     1775.035
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Range_ZEKRDZ_1996_1923.cif
_cod_data_source_block           O7S3Si2Yb4
_cod_database_code               8104158
Crystal structure of deuterides Tb3Ni6Al2Dx (x=0.3,0.5) based on intermetallic Tb3Ni6Al2 with Ca3Ag8 structural type
Yartys', V.A.; Pavlenko, V.V.; Khidirov, I.; Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR)) 18 (1992) 428–435; doi:

data_1536824
_publ_section_title
;
 Crystal structure of deuterides Tb3Ni6Al2Dx (x=0.3,0.5) based on
 intermetallic Tb3Ni6Al2 with Ca3Ag8 structural type
;
_journal_name_full
;
Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR))
;
_journal_page_first              428
_journal_page_last               435
_journal_volume                  18
_journal_year                    1992
_chemical_formula_sum            'Al2 D0.5 Ni6 Tb3'
_chemical_name_systematic        'Tb3 Ni6 Al2 D0.5'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.841
_cell_length_b                   9.841
_cell_length_c                   9.841
_cell_volume                     953.054
_citation_journal_id_ASTM        KOKHDC
_cod_data_source_file            Yartys_KOKHDC_1992_1345.cif
_cod_data_source_block           D0.5Al2Ni6Tb3
_cod_original_cell_volume        953.0543
_cod_original_formula_sum        'D0.5 Al2 Ni6 Tb3'
_cod_database_code               1536824
Role of bonding, reduced screening, and structure in the hightemperature superconductors
Falter, C.; Klenner, M.; Chen, Q.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 48 (1993) 16690–16706; doi:

data_1536825
_publ_section_title
;
 Role of bonding, reduced screening, and structure in the hightemperature
 superconductors
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              16690
_journal_page_last               16706
_journal_volume                  48
_journal_year                    1993
_chemical_formula_sum            'Ga N'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.985
_cell_length_b                   3.985
_cell_length_c                   3.985
_cell_volume                     63.283
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Falter_PRBMDO_1993_1896.cif
_cod_data_source_block           Ga1N1
_cod_original_cell_volume        63.28269
_cod_original_formula_sum        'Ga1 N1'
_cod_database_code               1536825
Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
Koenigstein, K.; Jansen, M.; Chemische Berichte 127 (1994) 1213–1218; doi:

data_1536826
_publ_section_title
;
 Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
;
_journal_name_full               'Chemische Berichte'
_journal_page_first              1213
_journal_page_last               1218
_journal_volume                  127
_journal_year                    1994
_chemical_formula_sum            'Cs2 H2 O14 P4 Si'
_chemical_name_systematic        'Cs2 H2 Si (P2 O7)2'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                94.99
_cell_angle_beta                 111.41
_cell_angle_gamma                113.2
_cell_formula_units_Z            2
_cell_length_a                   9.157
_cell_length_b                   9.219
_cell_length_c                   9.509
_cell_volume                     661.452
_citation_journal_id_ASTM        CHBEAM
_cod_data_source_file            Koenigstein_CHBEAM_1994_1301.cif
_cod_data_source_block           H2Cs2O14P4Si1
_cod_original_cell_volume        661.4519
_cod_original_formula_sum        'H2 Cs2 O14 P4 Si1'
_cod_database_code               1536826
Crystal structure of nickel lead selenide (3/2/2), Ni3 Pb2 Se2
Range, K.J.; Paulus, H.; Rau, F.; Zabel, M.; Zeitschrift fuer Kristallographie (149,1979-) 212 (1997) 136–136; doi:

data_8104159
_publ_section_title
;
 Crystal structure of nickel lead selenide (3/2/2), Ni3 Pb2 Se2
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              136
_journal_page_last               136
_journal_volume                  212
_journal_year                    1997
_chemical_formula_sum            'Ni3 Pb2 Se2'
_space_group_IT_number           166
_symmetry_space_group_name_Hall  '-R 3 2"'
_symmetry_space_group_name_H-M   'R -3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.6167
_cell_length_b                   5.6167
_cell_length_c                   14.286
_cell_volume                     390.305
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Range_ZEKRDZ_1997_1939.cif
_cod_data_source_block           Ni3Pb2Se2
_cod_original_cell_volume        390.3047
_cod_database_code               8104159
Crystal structure of Ti Fe1.16 V0.84 D1.9.
Yartys', V.A.; Mitrokhin, S.V.; Verbetskii, V.N.; Semenenko, K.N.; Zhurnal Neorganicheskoi Khimii 37 (1992) 32–37; doi:

data_1536827
_publ_section_title
;
 Crystal structure of Ti Fe1.16 V0.84 D1.9.
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              32
_journal_page_last               37
_journal_volume                  37
_journal_year                    1992
_chemical_formula_sum            'D1.9 Fe1.16 Ti V0.84'
_chemical_name_systematic        'Ti Fe1.16 V0.84 D1.9'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   5.067
_cell_length_b                   5.067
_cell_length_c                   8.28
_cell_volume                     184.104
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            Yartys_ZNOKAQ_1992_1247.cif
_cod_data_source_block           D1.9Fe1.16Ti1V0.84
_cod_original_cell_volume        184.1038
_cod_original_formula_sum        'D1.9 Fe1.16 Ti1 V0.84'
_cod_database_code               1536827
Role of bonding, reduced screening, and structure in the hightemperature superconductors
Falter, C.; Klenner, M.; Chen, Q.; Physical Review, Serie 3. B - Condensed Matter (18,1978-) 48 (1993) 16690–16706; doi:

data_1536828
_publ_section_title
;
 Role of bonding, reduced screening, and structure in the hightemperature
 superconductors
;
_journal_name_full
'Physical Review, Serie 3. B - Condensed Matter (18,1978-)'
_journal_page_first              16690
_journal_page_last               16706
_journal_volume                  48
_journal_year                    1993
_chemical_formula_sum            'In N'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.532
_cell_length_b                   4.532
_cell_length_c                   4.532
_cell_volume                     93.083
_citation_journal_id_ASTM        PRBMDO
_cod_data_source_file            Falter_PRBMDO_1993_1897.cif
_cod_data_source_block           In1N1
_cod_original_cell_volume        93.08286
_cod_original_formula_sum        'In1 N1'
_cod_database_code               1536828
Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
Koenigstein, K.; Jansen, M.; Chemische Berichte 127 (1994) 1213–1218; doi:

data_1536829
_publ_section_title
;
 Ein einfacher Weg zu Silicium in oktaedrischer Sauerstoffkoordination
;
_journal_name_full               'Chemische Berichte'
_journal_page_first              1213
_journal_page_last               1218
_journal_volume                  127
_journal_year                    1994
_chemical_formula_sum            'Ba H2 O14 P4 Si'
_chemical_name_systematic        'Ba H2 Si (P2 O7)2'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                75.34
_cell_angle_beta                 85.62
_cell_angle_gamma                75.76
_cell_formula_units_Z            1
_cell_length_a                   4.61
_cell_length_b                   6.595
_cell_length_c                   8.975
_cell_volume                     255.843
_citation_journal_id_ASTM        CHBEAM
_cod_data_source_file            Koenigstein_CHBEAM_1994_1310.cif
_cod_data_source_block           H2Ba1O14P4Si1
_cod_original_formula_sum        'H2 Ba1 O14 P4 Si1'
_cod_database_code               1536829
Mn Ga2 Se4 und Mn Ga2 Te4
Range, K.J.; Huebner, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (2,1947-32,1977) 31 (1976) 886–887; doi:

data_7222755
_publ_section_title
;
 Mn Ga2 Se4 und Mn Ga2 Te4
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (2,1947-32,1977)
;
_journal_page_first              886
_journal_page_last               887
_journal_volume                  31
_journal_year                    1976
_chemical_formula_sum            'Ga2 Mn Se4'
_chemical_name_systematic        'Mn Ga2 Se4'
_space_group_IT_number           82
_symmetry_space_group_name_Hall  'I -4'
_symmetry_space_group_name_H-M   'I -4'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.676
_cell_length_b                   5.676
_cell_length_c                   10.76
_cell_volume                     346.655
_citation_journal_id_ASTM        ZENBAX
_cod_data_source_file            Range_ZENBAX_1976_1894.cif
_cod_data_source_block           Ga2Mn1Se4
_cod_original_cell_volume        346.6547
_cod_original_formula_sum        'Ga2 Mn1 Se4'
_cod_database_code               7222755
Neutron diffraction study of deuteride Tb3 Ni6 Al2 D6.5
Yartys', V.A.; Khidirov, I.; Pavlenko, V.V.; Zhurnal Neorganicheskoi Khimii 37 (1992) 25–31; doi:

data_1536830
_publ_section_title
;
 Neutron diffraction study of deuteride Tb3 Ni6 Al2 D6.5
;
_journal_name_full               'Zhurnal Neorganicheskoi Khimii'
_journal_page_first              25
_journal_page_last               31
_journal_volume                  37
_journal_year                    1992
_chemical_formula_sum            'Al2 D6.5 Ni6 Tb3'
_chemical_name_systematic        'Tb3 Ni6 Al2 D6.5'
_space_group_IT_number           229
_symmetry_space_group_name_Hall  '-I 4 2 3'
_symmetry_space_group_name_H-M   'I m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.064
_cell_length_b                   9.064
_cell_length_c                   9.064
_cell_volume                     744.663
_citation_journal_id_ASTM        ZNOKAQ
_cod_data_source_file            Yartys_ZNOKAQ_1992_1248.cif
_cod_data_source_block           D6.5Al2Ni6Tb3
_cod_original_cell_volume        744.6629
_cod_original_formula_sum        'D6.5 Al2 Ni6 Tb3'
_cod_database_code               1536830
On the application of phase relationships to complex structures. XXIII. Automatic determination of crystal structures having pseudo-translational symmetry by a modified MULTAN procedure
Fan, H.-F.; Yao, J.-X.; Main, P.; Woolfson, M.M.; Acta Crystallographica C (39,1983-) 39 (1983) 566–569; doi:

data_2020160
_publ_section_title
;
 On the application of phase relationships to complex structures. XXIII.
 Automatic determination of crystal structures having pseudo-translational
 symmetry by a modified MULTAN procedure
;
_journal_name_full               'Acta Crystallographica C (39,1983-)'
_journal_page_first              566
_journal_page_last               569
_journal_volume                  39
_journal_year                    1983
_chemical_formula_sum            'C2 Ba Ce F O6'
_chemical_name_systematic        'Ba Ce F (C O3)2'
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   5.07
_cell_length_b                   5.07
_cell_length_c                   38.40799
_cell_volume                     855.004
_citation_journal_id_ASTM        ACSCEE
_cod_data_source_file            Fan_ACSCEE_1983_258.cif
_cod_data_source_block           C2Ba1Ce1F1O6
_cod_original_formula_sum        'C2 Ba1 Ce1 F1 O6'
_cod_database_code               2020160
Structural Investigations of Nasicon (Na1+x Zr2 Six P3-x O12; x=3) with X-Ray Diffraction at 298 K and 403K
Kohler, H.; Schulz, H.; Mel'nikov, O.K.; Materials Research Bulletin 18 (1983) 589–592; doi:

data_1536831
_publ_section_title
;
 Structural Investigations of Nasicon (Na1+x Zr2 Six P3-x O12; x=3) with
 X-Ray Diffraction at 298 K and 403K
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              589
_journal_page_last               592
_journal_volume                  18
_journal_year                    1983
_chemical_formula_sum            'Na4 O12 Si3 Zr2'
_chemical_name_systematic        'Na4 Zr2 (Si O4)3'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.193
_cell_length_b                   9.193
_cell_length_c                   22.289
_cell_volume                     1631.307
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Kohler_MRBUAC_1983_491.cif
_cod_data_source_block           Na4O12Si3Zr2
_cod_database_code               1536831
The chloro and bromo complexes of iridium(III) and iridium(IV). II. Structural chemistry of Ir(III) complexes
Rankin, D.A.; Australian Journal of Chemistry 36 (1983) 771–883; doi:

data_1536832
_publ_section_title
;
 The chloro and bromo complexes of iridium(III) and iridium(IV). II.
 Structural chemistry of Ir(III) complexes
;
_journal_name_full               'Australian Journal of Chemistry'
_journal_page_first              771
_journal_page_last               883
_journal_volume                  36
_journal_year                    1983
_chemical_formula_sum            'Cl6 H2 Ir K3 O'
_chemical_name_systematic        'K3 (Ir Cl6) H2 O'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.436
_cell_length_b                   15.682
_cell_length_c                   12.072
_cell_volume                     2354.298
_citation_journal_id_ASTM        AJCHAS
_cod_data_source_file            Rankin_AJCHAS_1983_686.cif
_cod_data_source_block           H2Cl6Ir1K3O1
_cod_original_formula_sum        'H2 Cl6 Ir1 K3 O1'
_cod_database_code               1536832
Crystal structure of tetrapotassium dihydrogen heptatungsteno tetramolybdeno monomanganese monoaquasilicate hydrate, K4 H2 (Si W7 Mo4 Mn (H2 O) O39) * 13(H2 O)
Ye, S.-R.; He, M.-Y.; Shan, Y.-K.; Dai Liyi; Zeitschrift fuer Kristallographie - New Crystal Structures 217 (2002) 451–452; doi:

data_8104160
_publ_section_title
;
 Crystal structure of tetrapotassium dihydrogen heptatungsteno
 tetramolybdeno monomanganese monoaquasilicate hydrate, K4 H2 (Si W7 Mo4
 Mn (H2 O) O39) * 13(H2 O)
;
_journal_name_full
;
Zeitschrift fuer Kristallographie - New Crystal Structures
;
_journal_page_first              451
_journal_page_last               452
_journal_volume                  217
_journal_year                    2002
_chemical_formula_sum            'H30 K4 Mn Mo4 O53 Si W7'
_chemical_name_systematic        'K4 H2 (Si W7 Mo4 Mn (H2 O) O39) (H2 O)13'
_space_group_IT_number           128
_symmetry_space_group_name_Hall  '-P 4 2n'
_symmetry_space_group_name_H-M   'P 4/m n c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.105
_cell_length_b                   14.105
_cell_length_c                   12.476
_cell_volume                     2482.113
_citation_journal_id_ASTM        ZKNSFT
_cod_data_source_file            Ye_ZKNSFT_2002_799.cif
_cod_data_source_block           H30K4Mn1Mo4O53Si1W7
_cod_original_formula_sum        'H30 K4 Mn1 Mo4 O53 Si1 W7'
_cod_database_code               8104160